Upcoming SlideShare
×

Fr3510071011

187 views

Published on

International Journal of Engineering Research and Applications (IJERA) is an open access online peer reviewed international journal that publishes research and review articles in the fields of Computer Science, Neural Networks, Electrical Engineering, Software Engineering, Information Technology, Mechanical Engineering, Chemical Engineering, Plastic Engineering, Food Technology, Textile Engineering, Nano Technology & science, Power Electronics, Electronics & Communication Engineering, Computational mathematics, Image processing, Civil Engineering, Structural Engineering, Environmental Engineering, VLSI Testing & Low Power VLSI Design etc.

0 Likes
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

Views
Total views
187
On SlideShare
0
From Embeds
0
Number of Embeds
1
Actions
Shares
0
3
0
Likes
0
Embeds 0
No embeds

No notes for slide

Fr3510071011

2. 2. P. Pratihar Int. Journal of Engineering Research and Application ISSN : 2248-9622, Vol. 3, Issue 5, Sep-Oct 2013, pp.1007-1011 Fig. 2: Based on projections, various areas. 2 ( A  R2 ) Drape Coefficent  100 %  ( R12  R2 2 ) where A  Area within the projectedoutline of the draped fabric, R 2  Radii of the disk, R1  Radii of the fabric sample The drape coefficient alone does not give a complete description of drape behaviour . There are many other aspects of the detailed form of draping. One other parameter which can easily be measured is the number of nodes formed as the fabric drapes. The following Fig. 3 illustrates how the number of nodes formed when the fabric bends symmetrically at the edge of the disc without double curvature and the number depends on the relative values of disc and fabric diameter. Flexible fabric will drape down by buckling into more folds than are shown in the Fig. 3 Fig.3: Influence of relative values of disc and fabric diameter on probable minimum number of nodes. (a) Specimen diameter 30 cm; disc diameter 15 cm – three nodes. (b) Specimen diameter 30 cm; disc diameter 21.3 cm – three nodes. Cusick [5] (1962) confirmed this experimentally and the following Fig. 4 based on his schematic representation of how the number of nodes depends on fabric stiffness and disc diameter. Fig. 4: Schematic representation of variation of number of nodes with disc diameter and fabric stiffness. Fabric diameter = 30 cm. www.ijera.com www.ijera.com Very stiff fabric merely sag slightly without forming any definite nodes: this gives the area designated as zero nodes. The number of nodes increases as the disc diameter decreases and the fabric stiffness decreases. There is general tendency for the number of nodes to decrease as drape coefficient rises. Same would be expected from the position of the disc diameter line in the fig above (Fig. 4). A given fabric does not always drape with same number of nodes. In his work Cusick [5] (1962) found that 60 tests on a cotton cambric gave the following distribution of results: 6 nodes, 5 tests 7 nodes, 22 tests 8 nodes, 24 tests 9 nodes, 9 tests The drape coefficient of the fabric was not much altered by differences in the number of nodes formed. The average value of drape coefficient with 6 nodes was 70% and with 9 nodes it was 72%. It is also possible to alter the number of nodes by disturbing the fabric. What this means is that there are a number of configurations where the energy passes through minimum values (corresponding to whole number of nodes) and the fabric does not necessarily fall in to the lowest of these configurations. B. Various Fabric Properties and Drape of Fabric From the discussions so far it can be seen that drape of fabric is a complex phenomena of various fabric properties like bending and buckling behaviour of fabric, shear properties, tensile properties, etc. Substantial amount of work has been done by various researchers and established lots of relationship between these parameters. Cusick [5,6,7] and Treloar [8] have done lots of work in this field and have investigated the dependence of drape of the fabric on bending and shear stiffness. According to Hearle [9], in his text book, “Structural Mechanics of Fibres, Yarns and Fabrics” ch. 12, the major mode of deformation in draping is fabric bending, but due to occurrence of double curvature, some shearing also takes place. Sharma [10] et al have studied on low-stress mechanical properties of fabric and its relationship with drapability characteristics of a fabric. In their work, they have observed that the drape coefficient has a strong correlation with bending properties, good to strong correlation with shearing properties and poor correlation with tensile properties. Nature of fabric deformation in drape is extremely important. The major mode of deformation in draping is fabric bending, but due to occurrence of double curvature some shearing also take place. Some tensile as well as compressive deformation also takes place, but as these are very small, can be ignored. Buckling behaviour also very important, but as it is related to bending stiffness, it will automatically be 1008 | P a g e
3. 3. P. Pratihar Int. Journal of Engineering Research and Application ISSN : 2248-9622, Vol. 3, Issue 5, Sep-Oct 2013, pp.1007-1011 taken care of along with bending length, as stiffness is a function of bending length. Therefore, it was said that bending and shear properties are the main factors influencing drape. Again, as the fabric is draping under its own weight, the measure of bending length by Shirley stiffness test method will be appropriate. The general pattern of behaviour were also estimated by a considerations of what happens when the shear stiffness takes extreme values i.e. zero shear stiffness and infinite shear stiffness, in the said book [9]. Work done by Okur [11] et al gives the prediction of fabric drape coefficient from FAST data. In their work, relationship between fabric drape coefficient obtained from Cusick’s drape meter and mechanical properties ascertained on the FAST system for women’s woven suiting fabrics were examined and a multiple linear regression model was proposed. Lai Sang-Song [12] had worked for establishing discriminant models of fabric characteristics. In the work four fabric groups, woven from cotton, linen, wool and silk were used. Discriminant analysis were used to characterize and discriminate between different fabric groups and 14 drape forms were able to classify the four groups of fabrics with a 98.3% classification accuracy rate. In another interesting work by Lo [13] et al, have presented a model for predicting fabric drape profiles using polar coordinates. It is claimed that with the help of their developed model, the drape coefficient, node locations, node numbers and node shape in the fabric drape profile can be predicted. In this work polar coordinate fitting is used to determine the constants and a good agreement was observed between the theoretical and experimental drape profiles and drape coefficient%. It was also claimed that drape profile can be directly predicted from bending and shear histeresis as constants in the drape profile model can be obtained by bending and shear histeresis using regression analysis. It was also suggested that for better prediction of the fabric drape profile, mean value should be taken in the warp, weft and ±45° directions than that in the warp and weft directions. III. www.ijera.com Fig. 5 : Using of Fabric as Long Skirt Fig. 6 : Using of Fabric as Short Skirt MODERN APPROACH - DYNAMIC DRAPE BEHAVIOUR OF FABRIC The drape measurement technique IS 8357:1977 gives a fair idea about drape coefficient of a fabric in static condition. But, when skirt is hanged to body its drape pattern changes as the body movement takes place (Fig. 5 & 6). Even a same fabric when used as table cloth, may form different drape pattern, when its position is disturbed (Fig. 7). Therefore, it is needed to evaluate fabric drape coefficient, when it’s static condition is disturbed. And also there is need to study what will be the drape coefficient after some movement in the fabric sample. This kind of study is called dynamic drape behavior study. www.ijera.com Fig. 7 : Using of Fabric as Table Cloth Quite a bit of work has been done on static drape behavior of fabric by Cusick in 60s. In 70s & 80s, it was felt that drape is not much important. Therefore the main focus during this period was on tensile behavior of the fabric. But during 90s, due to rapid growth of readymade garment along with computerized manufacturing system, it was felt by various research workers and market surveyors that drape is very important property one need to look in to for giving proper shape of a garment after it’s cutting and sewing. Moreover, to meet the customer requirement and stringent competition in the market 1009 | P a g e